DOI 10.1007/s10948-008-0440-y L E T T E R

**Muon-Spin Rotation Study of the Ternary Noncentrosymmetric**

**Superconductors Li**

**2**

**Pd**

**x**

**x**

**Pt**

**3**

**−x**

**−x**

**B**

**P.S. Häfliger· R. Khasanov · R. Lortz · A. Petrovi´c ·**
**K. Togano· C. Baines · B. Graneli · H. Keller**

Received: 10 December 2008 / Accepted: 15 December 2008 / Published online: 13 January 2009 © Springer Science+Business Media, LLC 2009

**Abstract We investigated the superconducting state of the**
noncentrosymmetric superconductors Li2Pd*x*Pt3*−x*B with
*superconducting transition temperature T*c *= 5.16(8) K*
*(x= 2.25), 3.56(8) K (x = 1.5) and 2.60 K (x = 0) by means*
of muon-spin rotation (µSR) and specific heat experiments.
*The µSR relaxation rate σ*scwas found to be constant at low
temperatures for all the compounds. Data taken at different
magnetic fields show that the magnetic penetration depth
*λ* is field-independent for Li2Pd*2.25*Pt*0.75*B and Li2Pt3B.
The electronic contribution to the specific heat measured in
Li2Pd*1.5*Pt*1.5*B and Li2Pt3B increases exponentially at the
*lowest temperatures. These features suggest that the whole*
*family of Li*2Pd*x*Pt3*−x*B comprises single-gap s-wave
super-conductors across the entire doping regime.

**Keywords Noncentrosymmetric superconductors**·
Magnetic penetration depth

P.S. Häfliger· B. Graneli · H. Keller

Physik-Institut der Universität Zürich, Winterthurerstrasse 190, 8057 Zürich, Switzerland

R. Khasanov (

)· C. BainesLaboratory for Muon-Spin Spectroscopy, Paul Scherrer Institute, CH-5232 Villigen PSI, Switzerland

e-mail:rustem.khasanov@psi.ch

R. Lortz· A. Petrovi´c

Département de Physique de la Matière Condensée de Genève, 24 quai Ernest-Ansermet, 1211 Geneva, Switzerland

K. Togano

National Institute for Materials Science, 1-2-1 Sengen, Tsukuba 305-0047, Japan

**1 Introduction**

Superconductivity in systems without inversion symmetry has recently attracted considerable interest, see e.g. [1,2]. The basic pairing states for a superconductor can be gener-ally classified as spin-singlet and spin-triplet states. Cooper pairing in the spin-singlet channel is based on time-reversal symmetry (Anderson’s theorem) [3], whereas for spin-triplet pairing also the existence of an inversion center in the crys-tal lattice is necessary [4]. However, the lack of an inversion center in the crystal lattice induces an antisymmetric spin– orbit coupling (ASOC) which is not destructive to special spin-triplet states as has been shown by Frigeri et al. [5] in the case of CePt3Si, for instance.

Lately the noncentrosymmetric superconductors Li2Pd3B
and Li2Pt3B have been discovered [6–9]. This system
presents an ideal playing field to study superconductivity
without inversion symmetry since there is no sign of
mag-netic order or strong electron correlation effects [6] such as
was found in CePt3Si, for instance. A significant effort was
put into identifying the superconducting state using various
experimental methods. While measurements of the
penetra-tion depth [10] and nuclear magnetic resonance (NMR)
ex-periments [11] suggest the existence of spin-triplet states
and nodes in the gap of Li2Pt3B, specific heat data
in-dicate conventional behavior as expected for an isotropic
*single-gap s-wave superconductor in Li*2Pd3B and Li2Pt3B
compounds [7]. Furthermore, our previous muon-spin
ro-tation (µSR) and magnetization experiments on Li2Pd3B
show no sign of an unconventional superconducting pairing
state [12,13].

In order to shed light on this controversy, we have
per-formed a systematic study of Li2Pd*x*Pt3*−x*B at different
*doping levels x choosing the bulk-sensitive transverse-field*

muon-spin rotation (TF-µSR) technique. Therewith we
in-vestigated the temperature and field dependence of the µSR
*relaxation rate σ in Li*2Pd*x*Pt3*−xB with x= 2.25, 1.5 and 0.*
In addition, we measured the low-temperature specific heat
of Li2Pd*1.5*Pt*1.5*B and Li2Pt3B.

**2 Experiments**

Li2Pd*x*Pt3*−x*B was prepared by two-step arc-melting [6] for
various doping concentrations. Details of the sample
prepa-ration can be found elsewhere [12]. The field-cooled
mag-netization of all the compounds was measured using a
su-perconducting quantum interference device (SQUID)
mag-netometer in fields ranging from 0.5 mT to 1.6 T at
temper-atures between 1.75 and 10 K. Specific heat was measured
from 6 down to 0.1 K.

*TF-µSR experiments were performed at the π M3 beam*
line at the Paul Scherrer Institute, Villigen, Switzerland. The
Li2Pd*x*Pt3*−xB (x= 2.25, 1.5 and 0) samples were *
*field-cooled from above T*cdown to 30 mK in fields of 0.1, 0.02
and 0.01 T. We performed temperature scans at low fields for
all the samples. Field-dependent data up to 1.5 T were taken
for Li2Pd*2.25*Pt*0.75*B and Li2Pt3B where each point includes
*a set of data at T > T*cand at 1 K after cooling in the field.

The µSR signal was recorded in the usual
time-differen-tial way by counting positrons from decaying muons as a
*function of time. The field distribution P (B) is then *
ob-tained from the Fourier transform of the measured time
*spectra P (t). P (t) is fitted with a Gaussian line and an *
os-cillatory term for the signal originating from the sample as
well as for the signal belonging to the sample holder (silver
plate). Figure1 *illustrates the P (t) and P (B) distributions*
inside the Li2Pt3B sample in the mixed state at 0.05 K after
being field-cooled in a magnetic field of 0.01 T. The
*sec-ond moment of P (B) is related to the µSR relaxation rate σ*
*which contains the superconducting component σ*sc as well
*as a contribution from the nuclear moments, σ*2*= σ*sc2*+ σ*n2.

**3 Results and Discussion**

In extreme type-II superconductors such as Li2Pd3B
*(Ginz-burg–Landau parameter κ*≈ 27 [12]), the magnetic field
*distribution P (B) is almost independent of the coherence*
*length ξ [*14*]. The magnetic penetration depth λ can then*
*be calculated from the known value of σ*sc using Brandt’s
formula describing the field variation in an ideal triangular
vortex lattice [15]:

*σsc*[m s−1]

*= 4.83 × 10*4_{(}_{1}_{− h)}_{1}_{+ 1.21}_{1}_{−}√* _{h}*3

*λ*−2[nm] (1)
*where h= H/H*c2*, with H*c2the upper critical field. Details
can be found elsewhere, see e.g. [12].

The magnetic field dependence of the second moment
*of σ*sc(1 K) for Li2Pd*2.25*Pt*0.75*B and Li2Pt3B is displayed
in the middle and right panels of Fig. 2, respectively. For
the sake of completeness we also show the field
*depen-dence of σ*sc*(0) for Li*2Pd3B [12] in the left panel. The
*data are taken at a fixed field at a temperature T > T*c,
the sample is then field-cooled to 1 K in order to
*deter-mine σ*sc *and σ*n unambiguously for each field. The
in-sets illustrate the corresponding temperature dependence of
*the upper critical field H*c2 as obtained from
magnetiza-tion (Li2Pd3B and Li2Pd*2.25*Pt*0.75*B) and specific heat
mea-surements (Li2Pt3B). Clearly Hc2*(T )* can be satisfactorily
fitted with the model based on the Werthamer–Helfand–
Hohenberg (WHH) theory [16], as demonstrated by the solid
*lines. The results for H*c2(*0) are listed in Table* 1*. H*c2 is
then inserted into (1*) in order to fit σ*sc(H ) to the
*exper-imental data with λ as a fit parameter. The results are in*
excellent agreement with the experimental data (shown by
*solid lines) implying that λ is field-independent. The *
*devia-tion at low fields (h≤ 0.003 in the case of Li*2Pd*2.25*Pt*0.75*B)
is expected since (1) is no longer valid at this region. In
the case of Li2Pt3B the error bars are large due to the

**Fig. 1 µSR time spectrum (left**

*panel) and magnetic field*

*distribution (right panel) of*
Li2Pt3*B taken in μ*0*H= 0.01 T*

below the superconducting transition temperature

*T*c*= 2.60 K (0.05 K). The lines*

represent a Gaussian fit as explained in the text

**Fig. 2 Field dependence of the**
µSR depolarization rate

*σ*sc*(T*= 1 K) in Li2Pd*x*Pt3−xB

*for x= 3 (left panel) [*12] as
*well as x= 2.25 (middle panel)*
*and 0 (right panel). The solid*
lines correspond to the results of
a least-squares fitting procedure
based on (1) as described in the
*text. In the insets the upper*
*critical field H*c2vs. temperature
*T* *is shown with the solid lines*
corresponding to a fit based on
the WHH model

**Table 1 Summary of the normal state and superconducting **
parame-ters for Li2Pd*x*Pt3*−x*B obtained in the present study from µSR
mea-surements. The meaning of the parameters is explained in the text

*x* *Tc*[K] *μ0Hc2[T] λ(0) [nm] κ(0)* *Δ0[meV] 2Δ*0/ kB*Tc*

3 *7.66(5)a 3.66(8)a* *252(2)a* *27(1)a 1.53(4)* 4.4(2)
2.25 5.16(8) 3.35(9) 413(8) 42(1) 1.03(4) 4.4(3)
1.5 3.56(8) 2.27(8) – – 0.59(2) 3.7(2)
0 2.60(5) 1.42(6) 608(10) 40(1) 0.41(2) 3.4(3)

*small value of the relaxation rate σ*sc. The resulting
*pene-tration depth λ(1 K) equals 413(8) nm and 608(10) nm for*
Li2Pd*2.25*Pt*0.75*B and Li2Pt3B, respectively, while we
*ob-tained λ(0)= 252(2) nm for Li*2Pd3B [12], see Table1. The
*value of λ(0) for Li*2Pd3B is in agreement with
magnetiza-tion measurements performed by Badica et al. [9], whereas
*our results for λ(0) for Li*2Pd*2.25*Pt*0.75*B and Li2Pt3B
devi-ate from those in [9].

*The superconducting coherence length ξ may be *
*es-timated from H*c2 *as ξ* *= [*0/(*2π H*c2)]*0.5*. We obtain
*ξ(0)* *= 9.5(2) nm (Li*2Pd3B) [12*], ξ(1 K)= 9.9(2) nm*
(Li2Pd*2.25*Pt*0.75*B) and 15.2(8) nm (Li2Pt3B). This results in
*a value for κ(0)= λ(0)/ξ(0) of 27(1) for Li*2Pd3B [12] with
*κ(1 K)= 42(1) and 40(1) for Li*2Pd*2.25*Pt*0.75*B and Li2Pt3B,
respectively (see Table1*). Since λ is constant at low *
*temper-atures as will be shown later, we may set ξ(0)≈ ξ(1 K) as*
*well as λ(0)≈ λ(1 K). The compounds in the present work*
are thus extreme type-II superconductors; µSR is therefore
an appropriate tool for penetration depth studies.

We also measured the temperature dependence of the
*µSR signal in order to extract λ*−2*(T )* using (1). The
re-sults are displayed in Fig. 3 for the entire doping series
Li2Pd*x*Pt3*−xB (x= 0, 1.5, 2.25 and 3 [*12]). The second
*moment of P (B) increases with x, and λ*−2*(x)*
monotoni-cally grows in turn with increasing Pd content. We observe
*that λ*−2*(T )* saturates at low temperatures and becomes

*T*-independent for all the compounds. This indicates that the
Fermi surface is fully gapped down to the lowest
*tempera-tures. Thus we applied a model for a BCS s-wave *
supercon-ductor in order to fit the data (see e.g. [17])

*λ*−2*(0)*
*λ*−2*(T )*= 1 + 2 ·
_{∞}
0
*dεdf*
*dE*
*.* (2)

Here*. . . represents an angular average over the Fermi *
*sur-face, f is the Fermi function and E*= *ε*2*+ |Δ|*2 the
*to-tal energy with ε the single-particle energy measured from*
the Fermi surface. Since we have assumed an isotropic
*gap, i.e. s-wave symmetry, the superconducting gap Δ is*
*k-independent, but only depends on temperature T such that*
*Δ(T )= Δ*0*· tanh(a*

√

*T*c*/T* *− 1) with a = 1.74 [18*]. The
*resulting gap values at zero temperature Δ*0are listed in
Ta-ble1*. Over the whole temperature range (T*cdown to 30 mK)
*and in the whole doping range (0≤ x ≤ 3) λ*−2is consistent
with what is expected for an isotropic BCS
superconduc-tor. However, the BCS fit to the Li2Pt3B data is not
satis-factory. In Li2Pt3B a considerable spin-triplet contribution
has previously been observed in [10,11], thus we assumed
a mixture of spin-triplet states associated with a strong
an-tisymmetric spin–orbit coupling resulting in two bands as
presented in [10]. Assuming the same set of parameters and
a BCS-temperature dependence of the superconducting gaps
(black dotted line in Fig.3*d), λ*−2*(T )*differs significantly
from our results. If we assume that the gap with nodes is
smeared out due to inhomogeneity of the sample, the
re-sulting model calculations are in agreement with our
exper-imental data, as illustrated by the solid black line in Fig.3d.
At this point we cannot exclude the existence of spin-triplet
states.

In order to clarify matters, the superconducting state
was also investigated by an independent study of the
spe-cific heat. Figure4illustrates the specific heat obtained for
Li2Pd*1.5*Pt*1.5*B (left panel) and Li2Pt3B (right panel) in zero

**Fig. 3 Temperature dependence**
*of λ*−2in Li2Pd*x*Pt3−xB for
*x= 3 at 0.02 T (black open*

*circles) and 0.5 T (black solid*
**circles) (panel a), 2.25 (panel**

* b), 1.5 (panel c) and 0 (panel d)*
at 0.01 T. The solid lines
correspond to a least-squares fit
to the experimental data for a

*BCS single-gap s-wave*superconductor based on (2) with the parameters given in the

*text. In panel d, the gray dashed*

*and dotted lines correspond to a*model based on a two-gap scenario where one and both bands become superconducting, respectively; see text for

*explanation. The inset of panel*

*b illustrates T*cas a function of

*Pd doping x*

**Fig. 4 Specific heat of**
Li2Pd*1.5*Pt*1.5B (left panel) and*

Li2Pt3*B (right panel)*

**Table 2 Summary of the**
normal state and

superconducting parameters for
Li2Pd*x*Pt3−xB obtained in the

present study from specific heat
measurements. The meaning of
the parameters is explained in
the text
*x* *T*c[K] *μ*0*H*c2[T] *γ* *ΔC/γ T*c *Δ*0 *2Δ*0*/ k*B*T*c
[mJ/gat K2_{]} _{[meV]}
3 *7.66(5)a* *3.66(8)a* *1.50(2)b* *2.0(3)b* *1.30(4)b* *3.94(4)b*
2.25 5.16(8) 3.35(9) – – – –
1.5 3.56(8) 2.27(8) 1.10(2) 1.28(3) 0.37(2) 3.3(2)
0 2.60(5) 1.42(6) 1.66(2) 1.75(2) 0.45(2) 4.0(2)

*field. The electronic contribution C*e*/T* to the specific heat
of Li2Pt3B, as obtained in a standard procedure by
quench-ing superconductivity in a field of 4 T, shows an exponential
increase at the lowest temperature. This is consistent with
our µSR data and therefore implies that Li2Pt3B is a fully
gapped superconductor. A fit using a standard single-gap
*s*-wave BCS model gives an excellent result (see Fig. 4).
*We obtain a gap-to-T*c *ratio of 2Δ*0*/ k*B*T*c*= 4.0(2) which*

is slightly larger than the µSR value but still in reasonable
*agreement. A smaller value of 2Δ*0/ kBTc*= 3.3(2) is *
de-rived for Li2Pd*1.5*Pt*1.5*B (see Table 2). A particularity of
Li2Pt3*B is a rather large residual Sommerfeld coefficient γr*.

A possible explanation is that within a two-gap scenario as presented by Yuan et al. [10] only one gap becomes super-conducting, while the gap with nodes is smeared out due to inhomogeneity of the sample. However, we have measured

another piece of the same large sample and we found a
*vari-ation of γr* of approximately 30%, but the superconducting

contribution remains unchanged. This behavior is typical for macroscopic metallic inclusions which remain in the normal state. Details of the specific heat measurements will be pub-lished elsewhere.

Interestingly, results in the literature postulate several
dif-ferent superconducting ground states for the Li2Pd*x*Pt3*−x*B
family. In particular, previous work on Li2Pt3B deviates
substantially from our conclusions. For instance, Yuan et
al. [10] found a linear temperature dependence of the
low-temperature penetration depth in Li2Pt3B by using a
tunnel-diode based, self-inductive technique. The results were
in-terpreted on the basis of a parity-mixed state with two Fermi
surfaces induced by the lack of inversion symmetry coupled
with a strong ASOC. The authors found that in Li2Pt3B one
of the superconducting gaps changes sign due to the
en-hanced ASOC, which leads to line nodes in the
supercon-ducting gap and therefore explains the non-saturating
pen-etration depth. None of our data—neither µSR nor specific
heat—supports such a scenario. We believe that the
differ-ence in the experimental data arises from the different
exper-imental techniques. In [10] data are taken by using a surface
sensitive technique with the magnetic field only
*penetrat-ing a distance λ below the surface (200–600 nm, see *
Ta-ble1). Muons, on the other hand, penetrate to much bigger
distances (fraction of millimeters) and therefore allow us to
study the magnetic penetration depth in the bulk. The
spe-cific heat is also a bulk-sensitive technique. Bearing these
in mind, the discrepancy between the results obtained in the
present study and those reported in [10] can be explained
by the difference between the bulk and the surface
proper-ties of Li2Pd*x*Pt3*−x*B, in analogy with what was observed
in conventional [19] and unconventional [20]
superconduc-tors. We would also like to emphasize that our data are in
excellent agreement with the specific heat data presented
in [7*]. Takeya et al. found values for 2Δ*0*/ k*B*T*c*= 3.94(4)*
and 3.53 for Li2Pd3B and Li2Pt3B, respectively, which are
in reasonable agreement with our results obtained from µSR
measurements.

We will briefly comment on the results of Nishiyama
et al. [11] obtained using the nuclear magnetic resonance
(NMR) technique which is also bulk-sensitive. They deduce
the existence of triplet states in Li2Pt3B from the Knight
*shift. However, it is not clear why they use a p-wave model*
to fit the data for the spin relaxation rate. Furthermore, they
*predict the behavior for an s-wave symmetry of the *
super-conducting gap in Li2Pt3B by using the value for the
super-conducting gap of Li2Pd3B which is more than three times
bigger, see Table 1. In addition, the absence of a Hebel–
Slichter peak in the spin relaxation does not necessarily
im-ply that the sample under investigation has an anisotropic
gap.

**4 Conclusions**

In conclusion, we have performed muon-spin rotation,
spe-cific heat and magnetization measurements on the ternary
boride superconductor Li2Pd*x*Pt3*−x*B. The main results are:
(i) the field dependence of the µSR relaxation rate is
*consis-tent with Brandt’s formula, (ii) the upper critical field H*c2
obeys the WHH model, (iii) the temperature dependence of
*λ*−2and (iv) the specific heat data are consistent with what
*is expected for an s-wave BCS superconductor. The *
*temper-ature dependence of λ*−2of Li2Pt3B can also be explained
by the existence of two bands induced by an ASOC where
only the one without nodes contributes to superconductivity
due to inhomogeneity of the sample. But specific heat data
indicate the existence of metallic inclusions. All our
mea-surements and analysis strongly point to a single isotropic
superconducting gap. No signature of an exotic
supercon-ducting order parameter was found. Thus we suggest that
*the whole family of Li*2Pd*x*Pt3*−x*B is a standard BCS
super-conductor with a single, isotropic gap.

**Acknowledgements** This work was partly performed at the Swiss
Muon Source (SµS), Paul Scherrer Institute (PSI, Switzerland). We
are grateful to N. Hayashi and M. Sigrist for helpful discussions as
well as to H. Takeya for providing us the samples Li2Pd*x*Pt3*−x*B,

*x= 3, 2.25, 1.5 and 0. This work was supported by the Swiss National*

Science Foundation and the K. Alex Müller Foundation.

**References**

1. Hayashi, N., Wakabayashi, K., Frigeri, P.A., Sigrist, M.: Phys.
**Rev. B 73, 024504 (2006)**

2. Bauer, E., Hilscher, G., Michor, H., Paul, Ch., Scheidt, E.W.,
Grib-anov, A., Seropegin, Yu., Nöel, H., Sigrist, M., Rogl, P.: Phys. Rev.
**Lett. 92, 027003 (2004)**

**3. Anderson, P.W.: J. Phys. Chem. Solids 11, 26 (1959)**
**4. Anderson, P.W.: Phys. Rev. B 30, 4000 (1984)**

5. Frigeri, P.A., Agterberg, D.F., Koga, A., Sigrist, M.: Phys. Rev.
**Lett. 92, 097001 (2004)**

6. Togano, K., Badica, P., Nakamori, Y., Orimo, S., Takeya, H.,
**Hi-rata, K.: Phys. Rev. Lett. 93, 247004 (2004)**

7. Takeya, H., Hirata, K., Yamaura, K., Togano, K., El Massalami,
**M., Rapp, R., Chaves, F.A., Ouladdiaf, B.: Phys. Rev. B 72,**
104506 (2005)

8. Badica, P., Kondo, T., Kudo, T., Nakamori, Y., Orimo, S.,
**Togano, K.: Appl. Phys. Lett. 85, 4433 (2004)**

**9. Badica, P., Kondo, T., Togano, K.: J. Phys. Soc. Jpn. 74, 1014**
(2005)

10. Yuan, H.Q., Agterberg, D.F., Hayashi, N., Badica, P., Vaderwelde,
**D., Togano, K., Sigrist, M., Salamon, M.B.: Phys. Rev. Lett. 97,**
017006 (2006)

**11. Nishiyama, M., Inada, Y., Zheng, G.-G.: Phys. Rev. Lett. 98,**
047002 (2007)

12. Khasanov, R., Landau, I.L., Baines, C., La Mattina, F.,
**Maisuradze, A., Togano, K., Keller, H.: Phys. Rev. B 73, 214528**
(2006)

**13. Landau, I.L., Khasanov, R., Togano, K., Keller, H.: Physica C 451,**
134 (2007)

**15. Brandt, E.H.: Phys. Rev. B 68, 054506 (2003)**

**16. Werthamer, N.R., Helfand, E., Hohenberg, P.C.: Phys. Rev. 147,**
295 (1966)

17. Kim, M.-S., Skinta, J.A., Lemberger, T.R., Kang, W.N., Kim,
**H.-J., Choi, E.-M., Lee, S.-I.: Phys. Rev. B 66, 064511 (2002)**
18. Bonalde, I., Yanoff, B.D., Salamon, M.B., Van Harlingen, D.J.,

**Chia, E.M.E., Mao, Z.Q., Maeno, Y.: Phys. Rev. Lett. 85, 4775**
(2000)

19. Khasanov, R., Di Castro, D., Paderno, Yu., Filippov, V., Brütsch,
**R., Keller, H.: Phys. Rev. B 72, 224509 (2005)**

20. Khasanov, R., Shengelaya, A., Bussmann-Holder, A., Karpinski,
**J., Keller, H., Müller, K.A.: J. Supercond. Nov. Magn. 21, 81**
(2008)